| ||Format||Pages||Price|| |
|3||$39.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$39.00||  ADD TO CART|
This practice provides an aid for setting up a suitable cleaning cycle preparatory to electroplating of low-carbon steel and indicates some of the precautions that must be taken to maintain this cycle in good operating condition. The preparatory procedure involves three basic steps in the following order: (1) removal of oils, grease, and caked-on dirt; (2) removal of scale and oxide films by pickling; and (3) removal of any smut left on the surface and activation of the steel. The cleaning of racked parts, which shall subsequently be electroplated in still tanks, agitated tanks, and semi- and full-automatic equipment, should be performed following this cycle: (1) precleaning; (2) electrocleaning; (3) water rinse; (4) acid pickling; (5) alkaline descaling; and (6) water rinse. Parts in bulk, which shall subsequently be electroplated in hand-operated or automatic barrels, should follow this cleaning cycle: (1) alkaline cleaning; (2) water rinse; (3) acid pickling; and (4) water rinse.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This practice is intended as an aid to electroplaters in setting up a suitable cleaning cycle preparatory to electroplating of low-carbon steel ( ) containing less than 0.35 mass % of carbon and to indicate some of the precautions that must be taken to maintain this cycle in good operating condition.
Note 1: The preparation of high-carbon steel for electroplating is covered in Guide .
1.2 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B242 Guide for Preparation of High-Carbon Steel for Electroplating
B322 Guide for Cleaning Metals Prior to Electroplating
ASTM B183-79(2014), Standard Practice for Preparation of Low-Carbon Steel for Electroplating, ASTM International, West Conshohocken, PA, 2014, www.astm.orgBack to Top